LMucko/crystallography-open-database huggingface dataset:
Crystal chemistry of sulfates from the Apuan Alps (Tuscany, Italy). V. Scordariite, K8(Fe3+0.67[]0.33)[Fe3+3O(SO4)6(H2O)3]2(H2O)11: A new metavoltine-related mineral
Biagioni, C.; Bindi, L.; Mauro, D.; Halenius; U; Minerals 9 (2019) –702; doi:

data_9017764
_publ_section_title
;
 Crystal chemistry of sulfates from the Apuan Alps (Tuscany, Italy).
 V. Scordariite, K8(Fe3+0.67[]0.33)[Fe3+3O(SO4)6(H2O)3]2(H2O)11:
 A new metavoltine-related mineral
;
_journal_name_full               Minerals
_journal_page_last               702
_journal_volume                  9
_journal_year                    2019
_chemical_compound_source        'Monte Arsiccio mine, Apuan Alps, Italy'
_chemical_formula_sum            'Fe6.66 H34 K7.5 Na0.5 O67 S12'
_chemical_name_mineral           Scordariite
_space_group_IT_number           148
_space_group_name_Hall           '-R 3'
_space_group_name_H-M_alt        'R -3 :H'
_symmetry_space_group_name_H-M   'R -3 :H'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            3
_cell_length_a                   9.7583
_cell_length_b                   9.7583
_cell_length_c                   53.687
_cell_volume                     4427.393
_database_code_amcsd             0020908
_exptl_crystal_density_diffrn    2.439
_cod_data_source_file            inputs/fixed/downloads/18/18728.cif
_cod_data_source_block           18728
_cod_original_sg_symbol_H-M      'R -3'
_cod_original_formula_sum        'K7.5 Na.5 Fe6.66 S12 O67 H34'
_cod_database_code               9017764
Crystal-chemistry of sulfates from the Apuan Alps (Tuscany, Italy). VII. Magnanelliite, K3Fe3+2(SO4)4 (OH)(H2O)2, a new sulfate from the Monte Arsiccio mine
Biagioni, C.; Bindi, L.; Kampf, A. R.; Minerals 9 (2019) –779; doi:

data_9017765
_publ_section_title
;
 Crystal-chemistry of sulfates from the Apuan Alps (Tuscany, Italy).
 VII. Magnanelliite, K3Fe3+2(SO4)4 (OH)(H2O)2, a new sulfate from the Monte Arsiccio mine
;
_journal_name_full               Minerals
_journal_page_last               779
_journal_volume                  9
_journal_year                    2019
_chemical_compound_source        'Monte Arsiccio mine, Apuan Alps, Italy'
_chemical_formula_sum            'Al0.156 Fe1.844 H5 K3 O19 S4'
_chemical_name_mineral           Magnanelliite
_space_group_IT_number           15
_space_group_name_Hall           '-C 2yc'
_space_group_name_H-M_alt        'C 1 2/c 1'
_symmetry_space_group_name_H-M   'C 1 2/c 1'
_cell_angle_alpha                90
_cell_angle_beta                 94.0640
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   7.5491
_cell_length_b                   16.8652
_cell_length_c                   12.1574
_cell_volume                     1543.953
_database_code_amcsd             0020909
_exptl_crystal_density_diffrn    2.847
_cod_data_source_file            inputs/fixed/downloads/18/18729.cif
_cod_data_source_block           18729
_cod_original_formula_sum        'K3 (Fe1.844 Al.156) S4 O19 H5'
_cod_database_code               9017765
Using complementary methods of synchrotron radiation powder diffraction and pair distribution functions to refine crystal structures with high quality parameters - A review Note: X-ray data, chemistry data provided by author
Lee, S.; Xu, H.; Minerals 10 (2020) –124; doi:

data_9017766
_publ_section_title
;
 Using complementary methods of synchrotron radiation powder diffraction and
 pair distribution functions to refine crystal structures with high quality
 parameters - A review
 Note: X-ray data, chemistry data provided by author
;
_journal_name_full               Minerals
_journal_page_last               124
_journal_volume                  10
_journal_year                    2020
_chemical_compound_source        'Murfreesboro, Arkansas, USA'
_chemical_formula_sum
'Al1.992 Ca0.012 Fe0.016 H4 Mg0.008 O9 Si1.956 Ti0.018'
_chemical_name_mineral           Kaolinite
_space_group_IT_number           1
_space_group_name_Hall           'C 1'
_space_group_name_H-M_alt        'C 1'
_symmetry_space_group_name_H-M   'C 1'
_cell_angle_alpha                91.704
_cell_angle_beta                 104.735
_cell_angle_gamma                89.852
_cell_formula_units_Z            2
_cell_length_a                   5.1546
_cell_length_b                   8.9425
_cell_length_c                   7.4033
_cell_volume                     329.882
_database_code_amcsd             0020861
_exptl_crystal_density_diffrn    2.609
_cod_data_source_file            inputs/fixed/downloads/18/18730.cif
_cod_data_source_block           18730
_cod_original_formula_sum
'Al1.992 Fe.016 Mg.008 Ca.012 Si1.956 Ti.018 O9 H4'
_cod_database_code               9017766
Using complementary methods of synchrotron radiation powder diffraction and pair distribution functions to refine crystal structures with high quality parameters - A review Note: Neutron data, chemistry data provided by author
Lee, S.; Xu, H.; Minerals 10 (2020) –124; doi:

data_9017767
_publ_section_title
;
 Using complementary methods of synchrotron radiation powder diffraction and
 pair distribution functions to refine crystal structures with high quality
 parameters - A review
 Note: Neutron data, chemistry data provided by author
;
_journal_name_full               Minerals
_journal_page_last               124
_journal_volume                  10
_journal_year                    2020
_chemical_compound_source        'Murfreesboro, Arkansas, USA'
_chemical_formula_sum
'Al1.992 Ca0.012 Fe0.016 H4 Mg0.008 O9 Si1.956 Ti0.018'
_chemical_name_mineral           Kaolinite
_space_group_IT_number           1
_space_group_name_Hall           'C 1'
_space_group_name_H-M_alt        'C 1'
_symmetry_space_group_name_H-M   'C 1'
_cell_angle_alpha                91.715
_cell_angle_beta                 104.756
_cell_angle_gamma                89.866
_cell_formula_units_Z            2
_cell_length_a                   5.1528
_cell_length_b                   8.9415
_cell_length_c                   7.3985
_cell_volume                     329.482
_database_code_amcsd             0020862
_exptl_crystal_density_diffrn    2.612
_cod_data_source_file            inputs/fixed/downloads/18/18731.cif
_cod_data_source_block           18731
_cod_original_formula_sum
'Al1.992 Fe.016 Mg.008 Ca.012 Si1.956 Ti.018 O9 H4'
_cod_database_code               9017767
Structure analysis of natural wangdaodeite - LiNbO3-type FeTiO3
Tschauner, O.; Ma, C.; Newville, M. G.; Lanzirotti, A.; Minerals 10 (2020) –1072; doi:

data_9017768
_publ_section_title
;
 Structure analysis of natural wangdaodeite - LiNbO3-type FeTiO3
;
_journal_name_full               Minerals
_journal_page_last               1072
_journal_volume                  10
_journal_year                    2020
_chemical_compound_source        'Ries impact structure, Germany'
_chemical_formula_sum            'Fe0.92 Mn0.08 O3 Ti'
_chemical_name_mineral           Wangdaodeite
_space_group_IT_number           148
_space_group_name_Hall           '-R 3'
_space_group_name_H-M_alt        'R -3 :H'
_symmetry_space_group_name_H-M   'R -3 :H'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_length_a                   5.148
_cell_length_b                   5.148
_cell_length_c                   13.649
_cell_formula_units_Z            6
_cell_volume                     313.263
_database_code_amcsd             0020928
_exptl_crystal_density_diffrn    4.823
_cod_data_source_file            inputs/fixed/downloads/18/18732.cif
_cod_data_source_block           18732
_cod_original_sg_symbol_H-M      'R -3'
_cod_original_formula_sum        '(Fe.92 Mn.08) Ti O3'
_cod_database_code               9017768
Rippite, K2(Nb,Ti)2(Si4O12)O(O,F), a new K-Nb-cyclosilicate from Chuktukon Carbonatite Massif, Chadobets Upland, Krasnoyarsk Territory, Russia
Sharygin, V. V.; Doroshkevich, A. G.; Seryotkin, Y. V.; Karmanov, N. S.; Belogub, E. V.; Moroz, T. N.; Nigmatulina, E. N.; Yelisseyev, A. P.; Vedenyapin, V. N.; Kupriyanov, I. N.; Minerals 10 (2020) –1102; doi:

data_9017769
_publ_section_title
;
 Rippite, K2(Nb,Ti)2(Si4O12)O(O,F), a new K-Nb-cyclosilicate from Chuktukon
 Carbonatite Massif, Chadobets Upland, Krasnoyarsk Territory, Russia
;
_journal_name_full               Minerals
_journal_page_last               1102
_journal_volume                  10
_journal_year                    2020
_chemical_compound_source        'Chuktukon Carbonatite Massif, Russia'
_chemical_formula_sum            'K Nb0.96 O7 Si2 Ti0.02 Zr0.01'
_chemical_name_mineral           Rippite
_space_group_IT_number           100
_space_group_name_Hall           'P 4 -2ab'
_space_group_name_H-M_alt        'P 4 b m'
_symmetry_space_group_name_H-M   'P 4 b m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   8.73885
_cell_length_b                   8.73885
_cell_length_c                   8.1277
_cell_formula_units_Z            4
_cell_volume                     620.692
_database_code_amcsd             0020927
_exptl_crystal_density_diffrn    3.192
_cod_data_source_file            inputs/fixed/downloads/18/18733.cif
_cod_data_source_block           18733
_cod_original_formula_sum        'Nb.96 Ti.02 Zr.01 K Si2 O7'
_cod_database_code               9017769
Kishonite, VH2, and oreillyite, Cr2N, two new minerals from the corundum xenocrysts of Mt Carmel, Northern Israel
Bindi, L.; Camara, F.; Gain, S. E. M.; Griffin, W. L.; Huang, J.; Saunders, M.; Toledo, V.; Minerals 10 (2020) –1118; doi:

data_9017770
_publ_section_title
;
 Kishonite, VH2, and oreillyite, Cr2N, two new minerals from the corundum
 xenocrysts of Mt Carmel, Northern Israel
;
_journal_name_full               Minerals
_journal_page_last               1118
_journal_volume                  10
_journal_year                    2020
_chemical_compound_source        'Mt Carmel, Israel'
_chemical_formula_sum            'Cr N0.47'
_chemical_name_mineral           Oreillyite
_space_group_IT_number           194
_space_group_name_Hall           '-P 6c 2c'
_space_group_name_H-M_alt        'P 63/m m c'
_symmetry_space_group_name_H-M   'P 63/m m c'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_length_a                   4.7853
_cell_length_b                   4.7853
_cell_length_c                   4.4630
_cell_formula_units_Z            2
_cell_volume                     88.507
_database_code_amcsd             0020923
_exptl_crystal_density_diffrn    2.198
_cod_data_source_file            inputs/fixed/downloads/18/18734.cif
_cod_data_source_block           18734
_cod_original_formula_sum        'Cr N.47'
_cod_database_code               9017770
Kishonite, VH2, and oreillyite, Cr2N, two new minerals from the corundum xenocrysts of Mt Carmel, Northern Israel
Bindi, L.; Camara, F.; Gain, S. E. M.; Griffin, W. L.; Huang, J.; Saunders, M.; Toledo, V.; Minerals 10 (2020) –1118; doi:

data_9017771
_publ_section_title
;
 Kishonite, VH2, and oreillyite, Cr2N, two new minerals from the corundum
 xenocrysts of Mt Carmel, Northern Israel
;
_journal_name_full               Minerals
_journal_page_last               1118
_journal_volume                  10
_journal_year                    2020
_chemical_compound_source        'Mt Carmel, Israel'
_chemical_formula_sum            'Al0.04 H2 V0.96'
_chemical_name_mineral           Kishonite
_space_group_IT_number           225
_space_group_name_Hall           '-F 4 2 3'
_space_group_name_H-M_alt        'F m -3 m'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   4.2680
_cell_length_b                   4.2680
_cell_length_c                   4.2680
_cell_formula_units_Z            4
_cell_volume                     77.745
_database_code_amcsd             0020924
_exptl_crystal_density_diffrn    4.443
_cod_data_source_file            inputs/fixed/downloads/18/18735.cif
_cod_data_source_block           18735
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_original_formula_sum        '(V.96 Al.04) H2'
_cod_database_code               9017771
Twinning, superstructure and chemical ordering in spryite, Ag8(As3+0.50As5+0.50)S6, at ultra-low temperature: An X-ray single-crystal study Note: T = 30 K
Bindi, L.; Morana, M.; Minerals 11 (2021) –286; doi:

data_9017772
_publ_section_title
;
 Twinning, superstructure and chemical ordering in spryite,
 Ag8(As3+0.50As5+0.50)S6, at ultra-low temperature: An X-ray single-crystal study
 Note: T = 30 K
;
_journal_name_full               Minerals
_journal_page_last               286
_journal_volume                  11
_journal_year                    2021
_chemical_compound_source
'Uchucchacua, Oyon district, Catajambo, Lima Department, Peru'
_chemical_formula_sum            'Ag24 As2 Ge S18'
_chemical_name_mineral           Spryite
_space_group_IT_number           33
_space_group_name_Hall           'P 2c -2n'
_space_group_name_H-M_alt        'P n a 21'
_symmetry_space_group_name_H-M   'P n a 21'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   14.866
_cell_length_b                   22.240
_cell_length_c                   10.3940
_cell_formula_units_Z            4
_cell_volume                     3436.463
_database_code_amcsd             0020943
_diffrn_ambient_temperature      30
_exptl_crystal_density_diffrn    6.549
_cod_data_source_file            inputs/fixed/downloads/18/18736.cif
_cod_data_source_block           18736
_cod_database_code               9017772
The compounds KAs4O6X (X=Cl,Br,I) and NH4As4O6X (X=Br,I): Hydrothermal syntheses and structure determinations
Pertlik, F.; Monatshefte fur Chemie 119 (1988) 451–456; doi:

data_9017773
_publ_section_title
;
 The compounds KAs4O6X (X=Cl,Br,I) and NH4As4O6X (X=Br,I):
 Hydrothermal syntheses and structure determinations
;
_journal_name_full               'Monatshefte fur Chemie'
_journal_page_first              451
_journal_page_last               456
_journal_volume                  119
_journal_year                    1988
_chemical_compound_source        Synthetic
_chemical_formula_sum            'As4 Br K O6'
_space_group_IT_number           177
_space_group_name_Hall           'P 6 2'
_space_group_name_H-M_alt        'P 6 2 2'
_symmetry_space_group_name_H-M   'P 6 2 2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            1
_cell_length_a                   5.257
_cell_length_b                   5.257
_cell_length_c                   8.955
_cell_volume                     214.325
_database_code_amcsd             0019950
_exptl_crystal_density_diffrn    3.988
_cod_data_source_file            inputs/fixed/downloads/18/18758.cif
_cod_data_source_block           18758
_cod_original_formula_sum        'K As4 O6 Br'
_cod_database_code               9017773
_amcsd_formula_title             KAs4O6Br
The thermal dehydration of magnesium aluminum pentafluoride dihydrate: crystal structures of MgAlF5(H2O)2 and MgAlF5
Weil, M.; Werner, F.; Monatshefte fur Chemie 132 (2001) 769–777; doi:

data_9017774
_publ_section_title
;
 The thermal dehydration of magnesium aluminum pentafluoride dihydrate:
 crystal structures of MgAlF5(H2O)2 and MgAlF5
;
_journal_name_full               'Monatshefte fur Chemie'
_journal_page_first              769
_journal_page_last               777
_journal_volume                  132
_journal_year                    2001
_chemical_compound_source        Synthetic
_chemical_formula_sum            'Al F5 Mg'
_space_group_IT_number           71
_space_group_name_Hall           '-I 2 2'
_space_group_name_H-M_alt        'I m m m'
_symmetry_space_group_name_H-M   'I m m m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   7.268
_cell_length_b                   6.123
_cell_length_c                   3.543
_cell_volume                     157.670
_database_code_amcsd             0020047
_exptl_crystal_density_diffrn    3.081
_cod_data_source_file            inputs/fixed/downloads/18/18763.cif
_cod_data_source_block           18763
_cod_original_formula_sum        'Mg Al F5'
_cod_database_code               9017774
_amcsd_formula_title             MgAlF5
Evidence of superdense aluminium synthesized by ultrafast microexplosion
Vailionis, A.; Gamaly, E. G.; Mizeikis, V.; Yang, W.; Rode, A. V.; Juodkazis, S.; Nature Communications 2 (2011) 445–446; doi:

data_9017775
_publ_section_title
;
 Evidence of superdense aluminium synthesized by ultrafast microexplosion
;
_journal_name_full               'Nature Communications'
_journal_page_first              445
_journal_page_last               446
_journal_volume                  2
_journal_year                    2011
_chemical_compound_source        Synthetic
_chemical_formula_sum            Al
_chemical_name_mineral           Steinhardtite
_space_group_IT_number           229
_space_group_name_Hall           '-I 4 2 3'
_space_group_name_H-M_alt        'I m -3 m'
_symmetry_space_group_name_H-M   'I m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   2.866
_cell_length_b                   2.866
_cell_length_c                   2.866
_cell_formula_units_Z            2
_cell_volume                     23.541
_database_code_amcsd             0020218
_exptl_crystal_density_diffrn    3.806
_cod_data_source_file            inputs/fixed/downloads/18/18805.cif
_cod_data_source_block           18805
_cod_database_code               9017775
Dumortierite, Si3B[Al6.75[]0.25O17.25(OH)0.75]: a detailed structure analysis
Moore, P. B.; Araki, T.; Neues Jahrbuch fur Mineralogie, Abhandlungen 132 (1978) 231–241; doi:

data_9017776
_publ_section_title
;
 Dumortierite, Si3B[Al6.75[]0.25O17.25(OH)0.75]: a detailed structure analysis
;
_journal_name_full               'Neues Jahrbuch fur Mineralogie, Abhandlungen'
_journal_page_first              231
_journal_page_last               241
_journal_volume                  132
_journal_year                    1978
_chemical_compound_source        'Saharina, Madagascar'
_chemical_formula_sum            'Al6.75 B H0.75 O18 Si3'
_chemical_name_mineral           Dumortierite
_space_group_IT_number           62
_space_group_name_Hall           '-P 2n 2a'
_space_group_name_H-M_alt        'P m c n'
_symmetry_space_group_name_H-M   'P m c n'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   11.828
_cell_length_b                   20.243
_cell_length_c                   4.7001
_cell_volume                     1125.365
_database_code_amcsd             0019939
_exptl_crystal_density_diffrn    3.340
_cod_data_source_file            inputs/fixed/downloads/18/18861.cif
_cod_data_source_block           18861
_cod_original_formula_sum        'Al6.75 Si3 B O18 H.75'
_cod_database_code               9017776
Low-temperature structures of orthoclase and sanidine Note: T = 121 K
Kimata, M.; Saito, S.; Shimizu, M.; Iida, I.; Matsui, T.; Neues Jahrbuch fur Mineralogie, Abhandlungen 171 (1996) 199–213; doi:

data_9017777
_publ_section_title
;
 Low-temperature structures of orthoclase and sanidine
 Note: T = 121 K
;
_journal_name_full               'Neues Jahrbuch fur Mineralogie, Abhandlungen'
_journal_page_first              199
_journal_page_last               213
_journal_volume                  171
_journal_year                    1996
_chemical_compound_source        'Itrongay, Madagascar'
_chemical_formula_sum            'Al K O8 Si3'
_chemical_name_mineral           Orthoclase
_space_group_IT_number           12
_space_group_name_Hall           '-C 2y'
_space_group_name_H-M_alt        'C 1 2/m 1'
_symmetry_space_group_name_H-M   'C 1 2/m 1'
_cell_angle_alpha                90
_cell_angle_beta                 116.07
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   8.574
_cell_length_b                   13.006
_cell_length_c                   7.191
_cell_volume                     720.307
_database_code_amcsd             0020548
_diffrn_ambient_temperature      121
_exptl_crystal_density_diffrn    2.567
_cod_data_source_file            inputs/fixed/downloads/18/18892.cif
_cod_data_source_block           18892
_cod_original_formula_sum        'K (Si3 Al) O8'
_cod_database_code               9017777
Low-temperature structures of orthoclase and sanidine Note: T = 296 K
Kimata, M.; Saito, S.; Shimizu, M.; Iida, I.; Matsui, T.; Neues Jahrbuch fur Mineralogie, Abhandlungen 171 (1996) 199–213; doi:

data_9017778
_publ_section_title
;
 Low-temperature structures of orthoclase and sanidine
 Note: T = 296 K
;
_journal_name_full               'Neues Jahrbuch fur Mineralogie, Abhandlungen'
_journal_page_first              199
_journal_page_last               213
_journal_volume                  171
_journal_year                    1996
_chemical_compound_source        'Itrongay, Madagascar'
_chemical_formula_sum            'Al K O8 Si3'
_chemical_name_mineral           Orthoclase
_space_group_IT_number           12
_space_group_name_Hall           '-C 2y'
_space_group_name_H-M_alt        'C 1 2/m 1'
_symmetry_space_group_name_H-M   'C 1 2/m 1'
_cell_angle_alpha                90
_cell_angle_beta                 116.03
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   8.600
_cell_length_b                   13.005
_cell_length_c                   7.193
_cell_volume                     722.883
_database_code_amcsd             0020549
_diffrn_ambient_temperature      296
_exptl_crystal_density_diffrn    2.557
_cod_data_source_file            inputs/fixed/downloads/18/18893.cif
_cod_data_source_block           18893
_cod_original_formula_sum        'K (Si3 Al) O8'
_cod_database_code               9017778
Low-temperature structures of orthoclase and sanidine Note: T = 121 K
Kimata, M.; Saito, S.; Shimizu, M.; Iida, I.; Matsui, T.; Neues Jahrbuch fur Mineralogie, Abhandlungen 171 (1996) 199–213; doi:

data_9017779
_publ_section_title
;
 Low-temperature structures of orthoclase and sanidine
 Note: T = 121 K
;
_journal_name_full               'Neues Jahrbuch fur Mineralogie, Abhandlungen'
_journal_page_first              199
_journal_page_last               213
_journal_volume                  171
_journal_year                    1996
_chemical_compound_source        'Volkesfeld, Eifel, Germany'
_chemical_formula_sum            'Al K O8 Si3'
_chemical_name_mineral           Sanidine
_space_group_IT_number           12
_space_group_name_Hall           '-C 2y'
_space_group_name_H-M_alt        'C 1 2/m 1'
_symmetry_space_group_name_H-M   'C 1 2/m 1'
_cell_angle_alpha                90
_cell_angle_beta                 116.03
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   8.514
_cell_length_b                   13.018
_cell_length_c                   7.183
_cell_volume                     715.374
_database_code_amcsd             0020560
_diffrn_ambient_temperature      121
_exptl_crystal_density_diffrn    2.584
_cod_data_source_file            inputs/fixed/downloads/18/18894.cif
_cod_data_source_block           18894
_cod_original_formula_sum        'K (Si3 Al) O8'
_cod_database_code               9017779